Thank you for visiting nature.com. You are using a browser version with limited support for CSS. To obtain the best experience, we recommend you use a more up to date browser (or turn off compatibility mode in Internet Explorer). In the meantime, to ensure continued support, we are displaying the site without styles and JavaScript.

# Gate tunable giant anisotropic resistance in ultra-thin GaTe

## Abstract

Anisotropy in crystals arises from different lattice periodicity along different crystallographic directions, and is usually more pronounced in two dimensional (2D) materials. Indeed, in the emerging 2D materials, electrical anisotropy has been one of the recent research focuses. However, key understandings of the in-plane anisotropic resistance in low-symmetry 2D materials, as well as demonstrations of model devices taking advantage of it, have proven difficult. Here, we show that, in few-layered semiconducting GaTe, electrical conductivity anisotropy between x and y directions of the 2D crystal can be gate tuned from several fold to over 103. This effect is further demonstrated to yield an anisotropic non-volatile memory behavior in ultra-thin GaTe, when equipped with an architecture of van der Waals floating gate. Our findings of gate-tunable giant anisotropic resistance effect pave the way for potential applications in nanoelectronics such as multifunctional directional memories in the 2D limit.

## Introduction

It is known that when electrically measuring a bulk material, the resulted conductivity may manifest strong directional dependencies1,2. Discrepancy of conductivity along different in-plane directions in layered bulk crystals can sometimes be as large as a few hundreds, which, however, often requires a certain conditions such as the presence of large external magnetic field3. Recently, low-symmetry 2D materials have attracted significant attentions because of the potential applications of in-plane anisotropic nanoelectronics4,5,6,7,8,9,10,11. For example, ultra-thin black phosphorous flake showed an in-plane anisotropic conductance reaching a ratio σa/σb of ~ 1.5, which in principle can be a direction-sensitive sensor4. ReS2 was reported to be another candidate for anisotropic 2D field effect transistor, which exhibited a σa of almost 10 times the value of σb9. Recent studies on GeP and GeAs flakes also showed anisotropic behavior with anisotropic factors of 1.5~2 for their conductance10,11.

To date, in-plane anisotropic factor Γa of electrical conductance in 2D materials is yet limited within one order of magnitude under ambient condition. It thus hinders future applications owing to a weak effective conductance difference between directions, and a larger anisotropic factor is highly desired. In this work, we show an observation of giant anisotropic resistance (GAR) behavior in few-layered p-type semiconducting GaTe. Among devices measured, the electrical conductivity ratio along x and y (x and y are defined in Fig. 1) directions of ultra-thin GaTe reaches an order of 103 at gate voltages close to the valence-band maximum (VBM), which can be further gate tuned down to < 10, upon hole doping. We show detailed analysis and physical understandings on the GAR effect. Based on this, floating gate anisotropic memory with directional multi-level outputs are demonstrated. Moreover, when measuring along fixed direction, the few-layered GaTe floating gate memory (FGM) exhibits On/Off ratio of 107 and retention time of 105 s, which is by far the best performance among FGMs made of 2D materials. Our findings open new possibilities toward next generation nanoelectronics, such as artificial neuron network based on anisotropic memory arrays.

## Results

### Characterizations of ultra-thin GaTe

Bulk GaTe single crystals were prepared via flux method and were confirmed via x-ray diffraction (see Supplementary Fig. 1). We mechanically exfoliated the bulk and deposited ultra-thin GaTe flakes onto 285 nm silicon oxide grown on heavily doped silicon wafers for optical and electrical characterizations. It is known that GaTe has a layered structure with lattice symmetry of group C2h (Fig. 1a), similar to that of 1 T′-MoTe2. The unit cell for a single layer GaTe is indicated in Fig. 1b. Monoclinic GaTe crystal is of very low symmetry, providing an ideal platform to study anisotropy12. It is also known as a typical p-type semiconductor with a direct band gap of ~ 1.65 eV13,14, which has many potential applications, such as photodetectors15, radiation detectors16, as well as thermophotovoltaic devices17. However, GaTe in air was reported to be easily oxidized18, leading to band gap restructuring in air, at the same time, the photoluminescence (PL) signal decreases and extra Raman peaks associated to oxides become more pronounced. Atomic Force Microscope (AFM) scan of a typical GaTe flake (14 nm in thickness) is shown in Fig. 1c, d. First, we characterized electronic transport of those flakes in air (Supplementary Figs. 26). However, without protection from air, the source-drain currents Ids of devices made by GaTe flakes are rather low, with maximum current of a few nano amperes, in agreement with other reported results19. It is found that, without thermal annealing, few-layered GaTe devices are barely conducting, as shown in Supplementary Fig. 2. In the following, we will focus on the devices made by ultra-thin GaTe flakes encapsulated by hexagonal boron nitride (h-BN) in a glove box, in order to diminish damages from air. Detailed analysis of the effect of h-BN protection can be found in Supplementary Figs. 711.

Polarized Raman can be used to determine crystal orientation in 2D flakes10,12, and also to deliver information of phonon modes that are related to the lattice symmetry. Supplementary Fig. 12 shows Raman spectra of a typical GaTe flake, with the angle-dependent intensity at Raman shift of 271.1 cm−1 plotted in a polar figure overlaid on the optical image shown in the inset. A twofold symmetry of the polar figure can be seen, with one of the polarized axis parallel to the exfoliated straight edge of the GaTe itself. Such a Raman-active mode is a Ag mode in C2h point group. From Raman tensor analysis, the direction of maximal Raman intensity of such Ag mode corresponds to the lattice direction with short lattice constant, defined as y direction in Fig. 1a, with x direction perpendicular to it. Raman mode at 164.6 cm−1 is another good reference for determining the crystalline direction (see Supplementary Fig. 13)12. Such a mode has a fourfold symmetry (Bg mode) and therefore four-lope angular dependence, with each lope 45 degrees away from the polarization axis of the mode at 271.1 cm−1. By comparing Raman anisotropy with the anisotropy of electrical conductivity (shown in the next section), it is known that y axis of GaTe layer corresponds to a maximum conductivity (Supplementary Figs. 1213). By this means, one can pattern electrodes for electrical measurements just with the zero angle defined along with such straight edges (y direction).

As shown in Fig. 1e, nine pairs of electrodes (20° angle between each two electrodes) were deposited onto the h-BN/GaTe/h-BN stack sample S1 (see Methods), which is further patterned into a circular shape in Fig. 1f. As a result, the source-drain current Ids along each pair of electrodes at gate voltage Vg = −80 V follows an ellipsoidal dependence of the testing angle, shown in Fig. 1g. It is rather straight forward that the maximum Ids flows in 0°, which is parallel to one of the straight edges, i.e., the y axis, as marked in Fig. 1f. Such twofold ellipsoidal oscillation of in-plane anisotropic conductivity is also seen in a number of other 2D materials4,5,9,10,11,20.

To unveil the origin of in-plane electrical conductivity anisotropy found in ultra-thin GaTe, we performed first-principles electronic structure and non-equilibrium Green’s functional quantum transport calculations with a simplified model on GaTe monolayer. Electronic band structure along high-symmetry lines is shown in Fig. 1h, with the first Brillouin zone and high-symmetry points defined in Fig. 1i. A direct band gap of 1.5 eV locates at the X point, in agreement with PL measurement in Supplementary Fig. 14. Thanks to the direct band gap, outstanding photo responses have been reported in GaTe devices15,21. What’s very interesting is the strongly anisotropic band dispersion obviously seen along two perpendicular directions (Γ–X and X–K). At the VBM, band dispersion along Γ–X is much bigger than along X–K, which gives rise to strong anisotropic effective mass m* at VBM, as shown in Supplementary Fig. 15. The calculated m* (shown in Supplementary Fig. 16) along X–K direction is ~ 10 times larger than that along Γ–X, which seems to lead to a better transport property along x axis than y axis. However, deformation potential E1 (shown in Supplementary Fig. 16) due to electron-phonon scattering shows an opposite trend to m* in both x and y axes, and dominates over the anisotropy of effective mass to give rise to the anisotropy of electrical conductivity σ according to the deformation potential theory (see Methods), σy is about five times as big as σx at low doping. When plotting experimental data in the renormalized conductivity polar figure in Fig. 1j, a twofold symmetry of conductance can be clearly seen.

### Gate-tunable GAR in ultra-thin GaTe

The above-mentioned twofold in-plane symmetry of resistivity can be reproduced in multiple GaTe devices (Supplementary Figs. 1718), and we performed a systematic study on the sample S2. As shown in Fig. 2a, with the same GaTe flake (optical image of the device is shown in the inset of Fig. 2a), field–effect curves, measured at source-drain voltage Vds = 2 V along x and y directions, exhibit strong anisotropy, indicated by red and blue colors, respectively. Ids measured along the 12 directions with a fixed Vds = 5 V are plotted at Vg = −60 V, while an ellipsoidal oscillation at all angles with 2π periodicity can be seen, shown in Fig. 2b. When the gate voltages were swept from −60 V to −30 V, the maximum-to-minimum Ids ratio of the ellipsoidal oscillation at each gate voltage varies largely. Note that similar gate-tunable anisotropic resistance behavior is also seen in bare GaTe devices without BN encapsulation (Supplementary Figs. 1920).

Taking y (0°) and x (90°) directions for examples, closer look of I–V output curves in the range of ±5 V is shown in Fig. 2c–d. It is seen that at high bias voltage, Ids for direction y is varying within 10−7 and 10−5 A, whereas Ids for direction x is varying within 10−11 and 10−6 A. We define the electrical maximum anisotropic ratio Γa as Iy/Ix for each fixed gate voltage. Strikingly, as extracted from Fig. 2b, Γa as a function of gate voltage shows a gate-tunability from less than one order to as large as 103. This gate-tunable GAR effect was not found in previous studies. We fabricated various samples in similar configuration of h-BN encapsulated ultra-thin GaTe devices (Supplementary Figs. 2123), with their Γa plotted together in Fig. 2e. In general, anisotropic ratio in those devices can be gate tuned from a few times, to several hundreds or even thousands folds, which is much higher than other 2D systems reported so far4,5,7,9,22. To push the 2D limit of the GaTe thicknesses studied in this work, we managed to fabricate sample of GaTe with ~ 4.8 nm in thickness. And as the inter-layer distance of GaTe is ~ 0.8 nm21, we can draw the conclusion that, down to the six-layer limit, the observed GAR prevails, as shown in Supplementary Fig. 24.

As Γa in ultra-thin GaTe is rather weak at relatively higher hole doping (say, in the Vg = −60 V limit), and becomes significantly enhanced close to the VBM in the vicinity of Vg = −30 V, it more or less shows a better electron collimation at higher Γa values, i.e., electrons tend to flow preferably along a certain direction at those conditions. Considering the deformation potential theory only applied to the band edge (VBM or CBM) and its inability to take care the gate-tunability on electronic transport23,24, we calculate I–V curves and their gate dependence by combining density functional theory (DFT) calculation with the non-equilibrium Green’s function (NEGF) method25 (see Methods), and show calculated field effect I-V data at Vds = 0.5 V along two perpendicular crystalline directions in Supplementary Fig. 25. To avoid possible contact Schottky barrier, we use p-type heavily doped GaTe as source and drain. I–V curves along both x and y directions show a similar behavior to the experimental ones as given in Fig. 2a. Iy,ds at Vds = 0.5 V increases from 1.39 μA at Vg = −9.1 V to 12.52 μA at Vg = −82 V. More strikingly is the gate dependence of Ix,ds, which changes by two orders of magnitude, from 4.63 × 10−3 μA at Vg = −9.1 V to 0.19 μA at Vg = −82 V. The calculated Iy/Ix ratio, given in filled red squares in Fig. 2e, decreases with increasing gate voltage, from ≈ 300 at −9.1 V to ≈60 at −82 V, agreeing qualitatively with the experimental ratio but in a milder way than the experimental data. The discrepancy can be ascribed to that extrinsic effect in experiment such as nonlinear contact resistivity is not taken into account in the simulated device. Nevertheless, the gate-tunable GAR can still be intrinsically analyzed from the calculated transmission coefficient, as shown in Supplementary Fig. 26. At low gate voltage (− 9.1 V), there is almost no x direction transmission channels in the scattering region between source energy level EL and drain energy level  ER, whereas a sizeable y direction transmission is observed, giving rise to a large anisotropic ratio Γa at low gate voltages. In contrast, at high gate voltage (− 82 V), non-zero transmission coefficient in channel material appears with comparable total transmission in both x and y directions, greatly suppressing GAR in GaTe.

### Ultra-thin GaTe anisotropic floating gate memory

It is of great importance to demonstrate conceptual devices taking advantage of the GAR effect in ultra-thin GaTe. In the following, we will discuss a prototype anisotropic memory based on ultra-thin GaTe. Using the vdW assembly method (see Methods), a few-layered graphene was equipped in addition to the h-BN/GaTe/h-BN sandwich, forming an architecture of FGM. Optical image and art view of such typical devices are shown in Fig. 3a, b.

Interestingly, when sweeping within the same gate window, the hysteresis memory curves along y and x directions vary largely, with a clear discrepancy of memory window size, shown in Fig. 3c, d. This result is more pronounced in a log scale when plotted together in Fig. 3e. One can see that after an operation of erasing (sweep the Vg from 0 V to −20 V, and back to 0 V), the device stays in an “Off” state in both directions. While an program operation (sweep the Vg from 0 V to 20 V, and back to 0 V), the device stays in two different “On” states in y and x directions, as indicated by colored circles in Fig. 3e, and their corresponding retention in Fig. 3f. It thus makes the device an anisotropic memory, i.e., one single operation of programming-erasing will generate two sets of data in the two directions, making the device conceptually compatible with direction-sensitive data storage.

## Discussion

To verify the performance of ultra-thin GaTe FGM with graphite floating gate along fixed direction, we recorded polarization gate voltages for different ranges from ±20 V to ±80 V in direction y, shown in Fig. 4a (see also Supplementary Figs. 2728). It can be seen that the GaTe memory shows rather stable erased state in all gate ranges. Once fed with the stimulation of pulsed Vg of ±40 V, the device can be readily erased and programmed as illustrated in Fig. 4b.

In the following, we compare the GaTe FGM with the state-of-the-art FGMs fabricated from other 2D materials26,27,28,29,30,31,32,33,34,35,36. Given that retention of the erased and/or programmed states is one of the most important parameter of such FGM, we recorded along direction y the on state (by a positive gate pulse), and the off state (by a negative gate pulse), respectively. Among GaTe FGM devices tested, the best performance (measured from sample S4 as shown in Fig. 4c) exhibits an on/off ratio exceeding 107 and the attenuation of the on/off ratio is < 5% in a retention time of 105 s (detailed memory characterizations of sample S4 are shown in Supplementary Fig. 29). By summarizing the state-of-the-art performance of FGM based on 2D materials, it is found that, our h-BN/GaTe/h-BN with graphite floating gate memory shows up to now the record on/off ratio and retention time, as shown in Fig. 4d. We attribute the observed high on/off ratio in the h-BN encapsulated devices to the better preserved band gap in the pristine GaTe. When the Fermi level is tuned to be inside the band gap (no electron density of state available), the off-state current is at the order of pA, whereas the on-state current reaches a few μA. To illustrate the working principle of the GaTe floating gate memory devices, we show, according to previous studies26,27,29,33, simplified band diagram in Supplementary Fig. 30.

In conclusion, we have discovered that ultra-thin GaTe encapsulated by h-BN devices show a twofold symmetry electrical conductance oscillations along different in-plane directions, with their maximum anisotropic ratios Iy/Ix gate-tunable in the range from < 10 to a few thousands. This GAR arises from the in-plane anisotropic transmission coefficients, and the anisotropic ratio can be changed by several orders of magnitude mainly owing to the sensitivity of x direction conduction channel to gating. Based on this GAR effect, we devised an anisotropic GaTe memory with a vdW assembled graphite floating gate. The prototype memory devices show direction-sensitive multiple-level output non-volatile memory behavior when measured from different directions. Moreover, fixed direction measurements suggest that the GaTe FGMs show record performances in terms of both on/off ratio and retention time among the state-of-the-art FGM based on 2D materials. Using this unit cell of GaTe anisotropic field effect transistor as a building block, it can be further expanded into many possible applications such as neural computation with GaTe FGM neural network arrays.

## Methods

Single crystal GaTe was prepared via the self-flux method. Raw bulk materials with stoichiometric ratio of Ga (purity 99.999%): Te (purity 99.9%) = 48.67:51.33 were mixed and kept at 880 °C for 5 h. The mixture was then cooled at the rate of 1.5 °C h−1, followed by a natural cooling process. The h-BN (crystals from HQ Graphene) encapsulated GaTe devices were fabricated using the dry-transfer methods (Supplementary Fig. 31)37, and then annealed in Ar:H2 (10:1) mixture at 320 °C for 30 mins before electrical measurements.

The h-BN-encapsulated GaTe heterostructures were fabricated in an mBraun-universe glove box. A Bruker Dimension Icon AFM was used for thicknesses and morphology tests. Raman measurements were performed by an HR 800 JobinYvon Horiba polarized Raman spectroscopy. The electrical performances of the devices were measured using a semiconductor analyzer (Agilent B1500A) and a probe station (Cascade Microtech Inc. EPS150) under ambient conditions.

The electronic band structure in this work was calculated by using the first-principles density functional theory as implemented in the VASP code38. Projector augmented wave pseudopotentials39 and the Perdew-Burke-Ernzerhof40 functional were, respectively, used to describe electron–ion interaction and electronic exchange-correlation interaction. We adopted 500 eV as the electronic kinetic energy cutoff for the plane-wave basis and 10−6 eV as the criterion for reaching self-consistency. The Brillouin zone (BZ) of the primitive unit cell (12 atoms per cell) was sampled by 20 × 20 × 1 k-points41. Rectangle supercell (24 atoms per cell) was used to calculate anisotropic electrical conductivity and the BZ was sampled by 2 × 6 × 1 k-points.

The electrical conductivity σ was evaluated based on σ = neμ, in which carrier mobility μ was calculated based upon the deformation potential theory with formula23,24

$$\mu = \frac{{e\hbar ^3C_{2D}}}{{k_BTm^ \ast m_dE_1^2}},$$
(1)

where is the reduced Planck constant, C2D is the elastic modulus derived from (E − E0)/A0 = 2/2 (E, E0, A0, C, and ε denote, respectively, the total energy, the total energy at equilibrium, the area of the 2D unit cell at equilibrium, elastic constant, and the lattice strain), kB is the Boltzmann constant, T is temperature, m* is the effective mass in the transport direction, md is the averaged effective mass defined by $$m_d = \sqrt {m_x^ \ast m_y^ \ast }$$ and E1 is the deformation potential constant of the VBM along the transport direction. E1 defined by E1 = ΔV/ε with ΔV as the energy change of the VBM under small strain ε.

I–V curve of the GaTe transistor was simulated using the DFT coupled with the NEGF method25, as implemented in the ATK package42. The structure of GaTe transistor is shown in Supplementary Fig. 25(a). We employed the Dirichlet boundary condition to ensure the charge neutrality in the source and the drain region. The temperature was set to 300 K. The density mesh cutoff was set to 80 Hartrees. The Monkhorst-Pack k-point meshes for device along the x and y direction were sampled with 40 × 6 × 1 and 114 × 6 × 1, respectively. Electron–ion interaction was treated by SG15 Optimized Norm-Conserving Vanderbilt (ONCV) pseudopotentials43,44. The transmission coefficient at energy E was averaged over 31 k-points perpendicular to the transport direction. The generalized gradient approximation was adopted for the electronic exchange-correction functional. The length of scattering region is 9.530 nm and 9.676 nm for transistor along x and y directions, respectively, both of which are sufficiently large to avoid interaction between source and drain. The code of VASP (www.vasp.at) and QuantumATK (https://docs.quantumwise.com/guides/guides.html) are commercially available from their official websites.

## Data availability

The data that support the findings of this study are available from the corresponding authors upon reasonable request.

## References

1. Krishnan, K. S. & Ganguli, N. Large anisotropy of the electrical conductivity of graphite. Nature 144, 667 (1939).

2. Eltsev, Y. et al. Anisotropic resistivity and hall effect in MgB2 single crystals. Phys. Rev. B 66, 180504(R) (2002).

3. Zhao, Y. et al. Anisotropic magnetictransport and exotic longitudinal linear magnetoresistance in WTe2 crystals. Phys. Rev. B 92, 041104(R) (2015).

4. Xia, F., Wang, H. & Jia, Y. Rediscovering black phosphorus as an anisotropic layered material for optoelectronics and electronics. Nat. Commun. 5, 4458 (2014).

5. Chen, Y. et al. Black arsenic: a layered semiconductor with extreme in-plane anisotropy. Adv. Mater. 30, 1800754 (2018).

6. Xu, X. et al. In-plane anisotropies of polarized raman response and electrical conductivity in layered tin selenide. ACS Appl. Mater. Interfaces 9, 12601–12607 (2017).

7. Liu, Y. et al. Raman signatures of broken inversion symmetry and in-plane anisotropy in type-II Weyl semmimetal candidate TaIrTe4. Adv. Mater. 30, 1706402 (2018).

8. Li, L. et al. Strong in-plane anisotropies of optical and electrical response in layered dimetal chalcogenide. ACS Nano 11, 10264–10272 (2017).

9. Liu, E. et al. Integrated digital inverters based on two-dimensional anisotropic ReS2 field-effect transistors. Nat. Commun. 6, 6991 (2015).

10. Li, L. et al. 2D GeP: An unexploited low-symmetry semiconductor with strong in-plane anisotropy. Adv. Mater. 30, 1706771 (2018).

11. Yang, S. et al. Highly in-plane optical and electrical anisotropy of 2D germanium arsenide. Adv. Funct. Mater. 28, 1707379 (2018).

12. Huang, S. et al. In-plane optical anisotropy of layered gallium telluride. ACS Nano 10, 8964–8972 (2016).

13. Sánchez-Royo, J. F. et al. Angle-resolved photoemission study and first-principles calculation of the electronic structure of GaTe. Phys. Rev. B 65, 115201 (2002).

14. Tatsuyama, C., Watanabe, Y., Hamaguchi, C. & Nakai, J. Some optical properties of layer-type semiconductor GaTe. J. Phys. Soc. Jpn. 29, 150 (1970).

15. Liu, F. et al. High-sensitivity photodetectors based on multilayer GaTe flakes. ACS Nano 8, 752–760 (2014).

16. Leão, C. R. & Lordi, V. Ab initio guided optimization of GaTe for radiation detection applications. Phys. Rev. B 84, 165206 (2011).

17. Rahmlow, T. D. Jr. et al. Development of front surface, spectral control filters with greater temperature stability for thermophotovoltaic energy conversion. AIP Conf. Proc. 890, 59 (2007).

18. Fonseca, J. J. et al. Bandgap restructuring of the layered semiconductor gallium telluride in air. Adv. Mater. 28, 6465–6470 (2016).

19. Hu, P. et al. Highly sensitive phototransistors based on two-dimensional GaTe nanosheets with direct bandgap. Nano Res. 7, 694–703 (2014).

20. Yang, S. X. et al. Highly-anisotropic optical and electrical properties in layered SnSe. Nano. Res. 11, 554–564 (2018).

21. Wang, Z. et al. Role of Ga vancancy on a multilayer GaTe phototransistor. ACS Nano 8, 4859–4865 (2014).

22. Qiu, G. et al. Observation of optical and electrical in-plane anisotropy in highmobility few-layer ZrTe5. Nano. Lett. 16, 7364–7369 (2016).

23. Bardeen, J. & Shockley, W. Deformation potentials and mobilities in non-polar crystals. Phys. Rev. 80, 72–80 (1950).

24. Dong, B. et al. New two-dimensional phase of tin chalcogenides: candidates for high-performance thermoelectric materials. Phys. Rev. Mater. 3, 013405 (2019).

25. Brandbyge, M., Mozos, J.-L., Ordejón, P., Taylor, J. & Stokbro, K. Density-functional method for nonequilibrium electron transport. Phys. Rev. B 65, 165401 (2002).

26. Li, D. et al. Nonvolatile floating-gate memories based on stacked black phosphorus-boron nitride-MoS2 heterostructures. Adv. Funct. Mater. 25, 7360–7365 (2015).

27. Gong, F. et al. High-sensitivity floating-gate phototransistors based on WS2 and MoS2. Adv. Funct. Mater. 26, 6084–6090 (2016).

28. Wang, J. et al. Floating gate memory-based monolayer MoS2 transistor with metal nanocrystals embedded in the gate dielectrics. Samll 11, 208–213 (2015).

29. Choi, M. S. et al. Controlled charge trapping by molybdenum disulphide and graphene in ultrathin heterostructured memory devices. Nat. Commun. 4, 1624 (2013).

30. Kang, M. et al. Stable charge storing in two-dimensional MoS2 nanoflake floating gates for multilevel organic flash memory. Nanoscale 6, 12315 (2014).

31. Vu, Q. A. et al. Two-terminal floating-gate memory with van der waals heterostructures for ultrahigh on/off ratio. Nat. Commun. 7, 12725 (2016).

32. Vu, Q. A. et al. A high-on/off-ratio floating-gate memristor array on a flexible substrate via CVD-grown large-area 2D layer stacking. Adv. Mater. 29, 1703363 (2017).

33. Bertolazzi, S., Krasnozhon, D. & Kis, A. Nonvolatile memory cells based on MoS2/graphene heterostructures. ACS Nano 7, 3246–3252 (2013).

34. Jang, S., Hwang, E., Lee, J. H., Park, H. S. & Cho, J. H. Graphene-graphene oxide floating gate transistor memory. Small 11, 311–318 (2015).

35. Jang, S., Hwang, E. & Cho, J. H. Graphene nano-floating gate transistor memory on plastic. Nanoscale 6, 15286 (2014).

36. Ji, Y. et al. Graphene quantum dots as a highly efficient solution-processed charge trapping medium for organic nano-floating gate memory. Nanotechnology 27, 145204 (2016).

37. Wang, Z. et al. Electric-field control of magnetism in a few-layered van der waals ferromagnetic semiconductor. Nat. Nanotechnol. 13, 554–559 (2018).

38. Kresse, G. & Furthmüller, J. Efficient iterative schemes for ab initio total-energy calculations using a plane-wave basis set. Phys. Rev. B 54, 11169–11186 (1996).

39. Kresse, G. & Joubert, D. From ultrasoft pseudopotentials to the projector augmented-wave method. Phys. Rev. B 59, 1758–1775 (1999).

40. Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized gradient approximation made simple. Phys. Rev. Lett. 77, 3865–3868 (1996).

41. Monkhorst, H. J. & Pack, J. D. Special points for brillouin-zone integrations. Phys. Rev. B 13, 5188–5192 (1976).

42. QuantumATK version 2018.06. Synopsys QuantumWise A/S, https://www.synopsys.com/silicon/quantumatk.html.

43. Hamann, D. R. Optimized norm-conserving vanderbilt pseudopotentials. Phys. Rev. B 88, 085117 (2013).

44. Schlipf, M. & Gygi, F. Optimization algorithm for the generation of oncv pseudopotentials. Comput. Phys. Commun. 196, 36–44 (2015).

## Acknowledgements

This work is supported by the National Key R&D Program of China (2017YFA0206302), and is supported by the National Natural Science Foundation of China (NSFC) with Grant 11504385 and 51627801. T. Yang acknowledges supports from the Major Program of Aerospace Advanced Manufacturing Technology Research Foundation NSFC and CASC, China (no. U1537204). L.T. Xiao acknowledges support from the National Key R&D Program of China (2017YFA0304203). H.H. Guo acknowledges NSFC Grant no. 51702146. Z. Han acknowledges the support from the Program of State Key Laboratory of Quantum Optics and Quantum Optics Devices (no. KF201816).

## Author information

Authors

### Contributions

Z.H., Z.Z. and T.Y. conceived the experiment and supervised the overall project. H.W., X.S., J.C. fabricated the devices. H.W., M.C., X.S., X.L., Y.Y. and Z.H. carried out electronic transport measurements; M.Z., C.Q., X.Z., L.X., J.Z., S.C. and J.C. carried out optical measurements; Y.W., B.D. and T.Y. conducted the theoretical simulations. J.H. and H.G. did the simulations on polarized Raman. D.S. contributed in sample fabrications. L.Z. and W.L. grew the GaTe bulk crystals. K.S., J.W. and Y.H. carried out TEM performances. The manuscript was written by Z.H., T.Y. and H.W. with discussion and inputs from all authors.

### Corresponding authors

Correspondence to Teng Yang, Chengbing Qin, Jianhao Chen or Zheng Han.

## Ethics declarations

### Competing interests

The authors declare no competing interests.

Journal peer review information: Nature Communications thanks the anonymous reviewer(s) for their contribution to the peer review of this work. Peer reviewer reports are available.

Publisher’s note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.

## Rights and permissions

Reprints and Permissions

Wang, H., Chen, ML., Zhu, M. et al. Gate tunable giant anisotropic resistance in ultra-thin GaTe. Nat Commun 10, 2302 (2019). https://doi.org/10.1038/s41467-019-10256-3

• Accepted:

• Published:

• DOI: https://doi.org/10.1038/s41467-019-10256-3

• ### Natural 2D layered mineral cannizzarite with anisotropic optical responses

• Arindam Dasgupta
• Xiaodong Yang
• Jie Gao

Scientific Reports (2022)

• ### Strong bulk-surface interaction dominated in-plane anisotropy of electronic structure in GaTe

• Kang Lai
• Sailong Ju
• Jiayu Dai

Communications Physics (2022)

• ### Highly in-plane anisotropy of thermal transport in suspended ternary chalcogenide Ta2NiS5

• Yue Su
• Chuyun Deng
• Xueao Zhang

Nano Research (2022)

• ### Flash memory based on MoTe2/boron nitride/graphene semi-floating gate heterostructure with non-volatile and dynamically tunable polarity

• Shijie Wang
• Guangyu Geng
• Jing Liu

Nano Research (2022)

• ### Thickness-dependent in-plane anisotropy of GaTe phonons

• Nguyen The Hoang
• Je-Ho Lee
• Maeng-Je Seong

Scientific Reports (2021)